Immobilization of Hexavalent Chromium Using Self-Compacting Soil Technology

A study of immobilization of hexavalent chromium in the form of Na2CrO4 salt by self-compacting soils (SCS) is presented. Carbofill E additive was used as SCS binder. The efficiency of immobilization of Cr (VI) was evaluated by washing out chromium compounds from SCS samples. The influence of the nature of the soil and the content of Carbofill E and Na2CrO4 in the SCS samples on the efficiency of Cr (VI) immobilization was studied. It was found that the nature of the soil and the content of Carbofill E in the SCS samples affect the immobilization of Cr (VI). Moreover, increasing the Carbofill E content in SCS samples further increases Cr (VI) immobilization. X-ray diffraction studies of the samples with immobilized hexavalent chromium showed that part of the sample transforms from a readily soluble form of salt into oxide forms of chromium and calcium-chromium, which are practically insoluble in water.


Introduction
Self-compacting soil mixture (SCS) is a highly flowable soil mixture prepared by homogeneous mixing of excavated loose soil, binder, and various additives. The mixture compacts its own weight and easily fills various excavations after formwork removal, cavities, and other hard-to-reach areas without the use of vibration. The technology for the production of SCS is in accordance with the principles of sustainable and environmentally friendly technology. By using SCS mixtures in the construction of buildings and roads, we conserve the natural resources of gravel/sand mixtures and it is possible to use excavated soil in the construction site for the same needs as we ordinarily use sand and gravel. Therefore, it is possible to recycle hardened SCS and make a product from it with new properties needed to implement design solutions. Heavy metals can be immobilized in SCS to permissible regulatory limits, thus providing a solution for contaminated soil remediation problems.
Industrialization and technological progress increase the release of hazardous waste, such as heavy metals, metalloids, and organic pollutants, into the environment [1,2]. Heavy metals are known to be significant environmental contaminants due to their high density and toxicity at low concentration. Furthermore, they cannot be decomposed into a nontoxic form. Most of the heavy metal concentration accumulates in the sediments of water basins and at the upper level of the soil. The main pathway of exposure to heavy metals for humans is food chain contamination [3,4]. Long-term contact with heavy metals causes major health problems in humans [5,6], animals [7], and plants [8]. Due to this, public health and environmental concerns are constantly raised. Therefore, it is imperative to reduce heavy metal pollution and the possibility of food contamination. Due to the widespread use of chromium in industrial processes, it is a major pollutant, among other toxic heavy metals.
compacting fillers based on excavated soil, tested recycled material or aggregates. The main Carbofill E binder compounds consisted of hatrurite (Ca 3 (SiO 4 )) and α-quartz SiO 2 , tricalcium aluminate (Ca 3 Al 2 O 6 ), gismondine (CaAl 2 Si 2 O 8 ·4 (H 2 O)), calcium sulfate (CaSO 4 ). The initial setting time (Vicat) of the Carbofill E mixture was 270 min., and the final setting time was 370 min. 43.5% water amount from cement mass was needed to prepare the paste of standard consistency. The flexural strength of the cement mortar with Carbofill E was 2.09 MPa after 3 days and 2.2 MPa after 28 days. The compressive strength of this cement mortar with Carbofill E was 26.5 MPa after 3 days and 46.2 MPa after 28 days.
For this study, clay and sandy soil were used from local construction sites in Lithuania. The sandy soil particles were sieved (according to EN 932-1), and their particle size distribution is given in Table 1. According to the results of granulometric composition tests of sandy soil, it is classified as poorly coarse sand according to EN ISO 14688-1.
The Atterberg limits (plastic limit, PL and liquid limit, LL) were found to determine the clay soil plasticity index according to EN ISO 17892-12. Variations of the Atterberg limits (the cone penetrometer method was used) of the clay are given in Table 2. The plasticity index (PI) is a measure of the plasticity of clay and according to the value of PI (25.36%) this clay could be assigned to highly plastic soils. The plasticity index (PI) is the difference between the liquid limit and the plastic limit (PI = LL−PL). The PI (>17) indicates highly plastic soil (based on EN ISO 14688-2). The water permeability of clay and sandy soils was determined according to EN ISO 17892-11. Permeability of raw soils: sandy soil-5 × 10 −5 m/s, and clay soil-5 × 10 −10 m/s. Soil pH was measured in a soil-water slurry. The procedure was performed according to ISO 10390 using a pH meter (Hanna instruments HI 98130). The average measurement results are sand pH-8.16, clay pH-7.98.
Organic matter content was determined after drying and combusting (450 • C) the samples according to EN 13039. The content of organic matter found in sand was 0.32% and 0.51% was found in clay. Therefore, we can say that there is no organic matter in the soil.

Methods
The mixing process was kept constant in the production of SCS to achieve the same homogeneity and uniformity in all the mixtures. It started by mixing all the soil and Carbofill E for one minute using a standard mixer as described in EN 12390-4. Then, three-quarters of the mixing water with Cr (VI) was added and mixed additionally for one minute. Thereafter, the required amount of water was added and the SCS was mixed additionally for approximately three minutes. After the mixing process was completed, the test was carried out on fresh SCS mortar to assess the diameter of the slump flow and the density of the mixture. The diameter of the slump flow was measured according to the procedure recommended by EN 12350-8. The diameter of the SCS mortar is measured in two perpendicular dimensions and the average is reported as the final diameter. The SCS mortars were proportioned to give a slump flow of 600 to 650 mm, which was achieved by using different water content. Between 5 × 10 2 and 1 × 10 5 mg Cr (VI) per kg of the mixture was added to the SCS samples during their formation. Na 2 CrO 4 salt dissolved in water was used as a source of Cr (VI). It was found that dissolved Cr (VI) had no effect on the physical-mechanical properties of the SCS.
The hardened SCS samples were also tested for compressive strength. Measurements were made after 7, 14, 28, 56, and 91 days, following the EN 12390-4 standard. Three 100 mm cubes were used for compressive strength tests. The cube samples were cast into the moulds without any compaction and vibration. After demoulding, all samples were kept at 20 ± 2 • C and 95% humidity until testing.
The permeability of hardened SCS samples was measured according to the procedure recommended by EN ISO 17892-11. Measurements were made after 28 days. The SCS samples were prepared as cylindrical samples (ø = 71,4 mm, H = 35 mm) without any compaction and vibration. All samples were stored at 20 ± 2 • C and 95% humidity until testing. The falling head test is performed when the test primers are poorly water-permeable (according to EN ISO 17892-11).
The washing out of Cr (VI) compounds from SCS samples was carried out in accordance with the recommendations of the standard EN 12457-2-2003. Two methods were used to bring the washing of Cr (VI) compounds as close as possible to real environment conditions. Method N 1 simulates the washout of undisturbed compacted soil. Here, the SCS cubes were continuously rinsed for 24 h in 10 L of distilled water circulated at 20 • C ( Figure 1). The water was then filtered through a 0.45 µm filter and the Cr (VI) content was determined. Method N 2 simulates the washing out of crushed soil. For this, the SCS cube was crushed and a grain fraction ≤4 mm was taken for further analysis. They were dried at 105 • C to constant weight and cooled to 20 • C; 50 g of these grains were placed in a conical flask filled with 500 mL of distilled water and shaken on a shaker at 200 rpm and 20 • C for 24 hours. The water used to wash the grains was analyzed as in the first method.
tionally for approximately three minutes. After the mixing process was complet test was carried out on fresh SCS mortar to assess the diameter of the slump flow density of the mixture. The diameter of the slump flow was measured according procedure recommended by EN 12350-8. The diameter of the SCS mortar is meas two perpendicular dimensions and the average is reported as the final diameter. T mortars were proportioned to give a slump flow of 600 to 650 mm, which was ac by using different water content. Between 5 × 10 2 and 1 × 10 5 mg Cr (VI) per kg mixture was added to the SCS samples during their formation. Na2CrO4 salt disso water was used as a source of Cr (VI). It was found that dissolved Cr (VI) had no e the physical-mechanical properties of the SCS.
The hardened SCS samples were also tested for compressive strength. Measur were made after 7, 14, 28, 56, and 91 days, following the EN 12390-4 standard. Th mm cubes were used for compressive strength tests. The cube samples were cast moulds without any compaction and vibration. After demoulding, all samples we at 20 ± 2 °C and 95% humidity until testing.
The permeability of hardened SCS samples was measured according to the dure recommended by EN ISO 17892-11. Measurements were made after 28 da SCS samples were prepared as cylindrical samples (ø = 71,4 mm, H = 35 mm) with compaction and vibration. All samples were stored at 20 ± 2 °C and 95% humidi testing. The falling head test is performed when the test primers are poorly waterable (according to EN ISO 17892-11).
The washing out of Cr (VI) compounds from SCS samples was carried out in ance with the recommendations of the standard EN 12457-2-2003. Two method used to bring the washing of Cr (VI) compounds as close as possible to real enviro conditions. Method N 1 simulates the washout of undisturbed compacted soil. H SCS cubes were continuously rinsed for 24 h in 10 L of distilled water circulated a ( Figure 1). The water was then filtered through a 0.45 µ m filter and the Cr (VI) was determined. Method N 2 simulates the washing out of crushed soil. For this, cube was crushed and a grain fraction ≤4 mm was taken for further analysis. The dried at 105 °C to constant weight and cooled to 20 °C ; 50 g of these grains were pl a conical flask filled with 500 mL of distilled water and shaken on a shaker at 200 r 20 °C for 24 hours. The water used to wash the grains was analyzed as in the first m The total amount of chromium in the water washed out from the SCS samples was determined by using the atomic absorption spectrometer (AAS) AA-7000 Shimadzu (Japan) (featuring λ= 357.9 nm) equipped with an electrodeless discharge lamp and an air-acetylene flame. For the conditions described above, the sensitivity of the AAS method is~0.2 µg/mL chromium for 1% absorption [40].

Physical and Mechanical Research of the SCS
The test results relevant to the diameter of the slump flow and the density of the mixtures are presented in Table 3. All SCS mixtures were designed to reach a diameter of the slump flow of 600-650 mm, which was acquired by adjusting the dose of water used. The compressive strength test results of different mixture compositions are shown in determined by using the atomic absorption spectrometer (AAS) AA-7000 Shimadzu (Japan) (featuring λ= 357.9 nm) equipped with an electrodeless discharge lamp and an airacetylene flame. For the conditions described above, the sensitivity of the AAS method is ~0.2 µ g/mL chromium for 1% absorption [40].

Physical and Mechanical Research of the SCS
The test results relevant to the diameter of the slump flow and the density of the mixtures are presented in Table 3. All SCS mixtures were designed to reach a diameter of the slump flow of 600-650 mm, which was acquired by adjusting the dose of water used. The compressive strength test results of different mixture compositions are shown in          The water permeability of hardened SCS with sandy and clay soils is shown in Figure  5. The coefficient of permeability of SCS mixed with sand and 10 %, 15%, 20% Carbofill E was found to vary between 4.28 × 10 −8 m/s and 2.04 × 10 −11 m/s, while the coefficient of permeability of SCS mixed with clay and 10 %, 15%, 20% Carbofill E was found to vary between 4.56 × 10 −10 m/s and 3.84 × 10 −10 m/s.  The water permeability of hardened SCS with sandy and clay soils is shown in Figure 5. The coefficient of permeability of SCS mixed with sand and 10 %, 15%, 20% Carbofill E was found to vary between 4.28 × 10 −8 m/s and 2.04 × 10 −11 m/s, while the coefficient of permeability of SCS mixed with clay and 10 %, 15%, 20% Carbofill E was found to vary between 4.56 × 10 −10 m/s and 3.84 × 10 −10 m/s.

Immobilization Studies of SCS Contaminated Cr (VI)
The research was carried out on the sandy and clay soils most widespread in Lithuania. Since the excavated sites in landscaped plots can be improved with SCS in the future, it is important that heavy metals are securely immobilized and their leeching from these soils is minimized. Initially, the effect of Carbofill E additive on the washing out of chromium compounds from SCS samples was evaluated. The Cr (VI) content in the samples exceeded the allowed hygienic standards (3000 mg/kg) by 30 times [41], and the content of Carbofill E additive ranged from 10% to 20%. Compared with other studies [42] , the same amount of the additions in blended cement pastes, which contain 15-20% bagasse ash, can be used effectively for the immobilization of concentrated waste Cr(VI) solutions. The data presented in Figures 6 and 7 show that the addition of Carbofill E dramatically reduces the washing out of chromium from all modified soil samples. For example, only 18.0 and 64.6 mg/kg of chromium were washed out from crushed sandy and clay SCS samples with 10% Carbofill E, respectively (Figures 6b and 7b). Meanwhile, the amount of chromium compounds washed out from uncrushed SCS soil samples decreased hundreds of times to 5.87 × 10 −2 and 6.89 × 10 −2 mg/kg, respectively (Figures 6a and 7a). A further increase in the Carbofill E content in the SCS samples further reduced the chromium washing out, although not as noticeably. For example, an increase in the concentration of Carbofill E in uncrushed sandy SCS samples from 10% to 15 % reduced the washing of chromium by approximately 9 times (from 5.87 × 10 −2 to 0.65 × 10 −2 mg/kg) and more than 16 times (from 18.0 to 1.1 mg/kg) in crushed samples. An increase in the amount of Carbofill E up to 20% in sandy SCS reduced the washing out of chromium from both soil samples only 1.86 times: from 0.65 × 10 −2 to 0.35 × 10 −2 mg/kg in uncrushed samples and 1.1 up to 0.591 mg/kg in crushed samples, respectively. The same dependence, only with a relatively large washing out of chromium, was observed for clay SCS samples ( Figure  7). The higher efficiency of chromium immobilization in sandy soil compared to clay soil is due to its higher density ( Figure 4). As a result, the water permeability of the soil decreases, which leads to a decrease in the leaching of chromium from sandy soil ( Figure 5).

Immobilization Studies of SCS Contaminated Cr (VI)
The research was carried out on the sandy and clay soils most widespread in Lithuania. Since the excavated sites in landscaped plots can be improved with SCS in the future, it is important that heavy metals are securely immobilized and their leeching from these soils is minimized. Initially, the effect of Carbofill E additive on the washing out of chromium compounds from SCS samples was evaluated. The Cr (VI) content in the samples exceeded the allowed hygienic standards (3000 mg/kg) by 30 times [41], and the content of Carbofill E additive ranged from 10% to 20%. Compared with other studies [42], the same amount of the additions in blended cement pastes, which contain 15-20% bagasse ash, can be used effectively for the immobilization of concentrated waste Cr(VI) solutions. The data presented in Figures 6 and 7 show that the addition of Carbofill E dramatically reduces the washing out of chromium from all modified soil samples. For example, only 18.0 and 64.6 mg/kg of chromium were washed out from crushed sandy and clay SCS samples with 10% Carbofill E, respectively (Figures 6b and 7b). Meanwhile, the amount of chromium compounds washed out from uncrushed SCS soil samples decreased hundreds of times to 5.87 × 10 −2 and 6.89 × 10 −2 mg/kg, respectively (Figures 6a and 7a). A further increase in the Carbofill E content in the SCS samples further reduced the chromium washing out, although not as noticeably. For example, an increase in the concentration of Carbofill E in uncrushed sandy SCS samples from 10% to 15 % reduced the washing of chromium by approximately 9 times (from 5.87 × 10 −2 to 0.65 × 10 −2 mg/kg) and more than 16 times (from 18.0 to 1.1 mg/kg) in crushed samples. An increase in the amount of Carbofill E up to 20% in sandy SCS reduced the washing out of chromium from both soil samples only 1.86 times: from 0.65 × 10 −2 to 0.35 × 10 −2 mg/kg in uncrushed samples and 1.1 up to 0.591 mg/kg in crushed samples, respectively. The same dependence, only with a relatively large washing out of chromium, was observed for clay SCS samples (Figure 7). The higher efficiency of chromium immobilization in sandy soil compared to clay soil is due to its higher density (Figure 4). As a result, the water permeability of the soil de-creases, which leads to a decrease in the leaching of chromium from sandy soil ( Figure 5). Since 10% Carbofill E in the sandy and clay SCS samples is sufficient to immobili Cr (VI), further studies were performed on samples with 10% of this binder. The sand samples of SCS with immobilized Cr (VI) content exceeding the permissible level from to 1000 times have been investigated. As can be seen from the graphs in Figure 8, t maximum chromium content (589.61 mg/kg) was washed out only from the crushed sam ple, which had a maximum chromium content (10 5 mg/kg) (Figure 8b). Meanwhile, ev at such high levels of chromium, only 9.58 mg/kg was washed out from the undisturb SCS sample. Since 10% Carbofill E in the sandy and clay SCS samples is sufficient to immobili Cr (VI), further studies were performed on samples with 10% of this binder. The sand samples of SCS with immobilized Cr (VI) content exceeding the permissible level from to 1000 times have been investigated. As can be seen from the graphs in Figure 8, t maximum chromium content (589.61 mg/kg) was washed out only from the crushed sam ple, which had a maximum chromium content (10 5 mg/kg) (Figure 8b). Meanwhile, ev at such high levels of chromium, only 9.58 mg/kg was washed out from the undisturb SCS sample. Since 10% Carbofill E in the sandy and clay SCS samples is sufficient to immobilize Cr (VI), further studies were performed on samples with 10% of this binder. The sandy samples of SCS with immobilized Cr (VI) content exceeding the permissible level from 5 to 1000 times have been investigated. As can be seen from the graphs in Figure 8, the maximum chromium content (589.61 mg/kg) was washed out only from the crushed sample, which had a maximum chromium content (10 5 mg/kg) (Figure 8b). Meanwhile, even at such high levels of chromium, only 9.58 mg/kg was washed out from the undisturbed SCS sample. Since 10% Carbofill E in the sandy and clay SCS samples is sufficient to immobilize Cr (VI), further studies were performed on samples with 10% of this binder. The sandy samples of SCS with immobilized Cr (VI) content exceeding the permissible level from 5 to 1000 times have been investigated. As can be seen from the graphs in Figure 8, the maximum chromium content (589.61 mg/kg) was washed out only from the crushed sam ple, which had a maximum chromium content (10 5 mg/kg) (Figure 8b). Meanwhile, even at such high levels of chromium, only 9.58 mg/kg was washed out from the undisturbed SCS sample.  The effectiveness of immobilization of heavy metals in SCS soils can be better illustrated not by the absolute amount of washed-out metals, but by the percentage of heavy metals remaining in these soils after the washing out procedure of the total amount added to them. Data in Table 4 show that the nature of the soil affects the immobilization of Cr (VI) only in crushed SCS samples with a 10% addition of Carbofill E. Meanwhile, in uncrushed soil samples, regardless of the nature of the soil and the amount of Carbofill E, more than 99.99% of the total added Cr (VI) content (3000 mg/kg) was immobilized. In sandy SCS samples with 10% Carbofill E and the maximum Cr (VI) content (10 5 mg/kg), the immobilization efficiency did not change: it was more than 99.99% in the uncrushed sample and 99.4% in the crushed sample. Studies showed that Carbofill E supplementation has an inhibitory effect on the immobilization of Cr (VI) in SCS. Meanwhile, the nature of the soil insignificantly affects the immobilization of Cr (VI) only in the samples of crushed soil.

X-ray Diffraction Studies of SCS Contaminated Cr (VI)
To understand the nature of the immobilization of Cr (VI) compounds in SCS, XRD analysis of these soils was carried out. This is a nondestructive method of instrumental analysis, which is informative and suitable for characterizing the crystal structure of materials; therefore, it is widely used in the study of inorganic crystalline compounds (silicates and other minerals, ceramics, cement and its hydration products, zeolites). The results of the study are presented in Figures 9 and 10, and the peaks of the identified compounds and their positions are tabulated in Supplementary Material Tables S1-S5. As expected, typical diffraction peaks for hexagonal quartz SiO 2 (83-539) prevail in all investigated samples of sandy SCS (Figure 9). Furthermore, their number and intensity decrease with increasing concentration of the additive (Tables S1-S3). Also, two peaks CaSiO 3 (84-655) and Ca 3 (Si 3 O 9 ) (76-1846) of composite monoclinic deformations of wollastonite 2M were found. These compounds were introduced into the SCS sample together with the Carbofill E binder. At the same time, Cr (VI) was not detected in the form of Na 2 CrO 4 . It is likely that part of this salt in SCS samples initially reacts in an alkaline medium with Ca 2+ ions present there, forming sparingly soluble CaCrO 4 calcium chromate according to Equation (1): Furthermore, redox reactions take place in which sparingly soluble and less oxidized chromium compounds are formed. The part of hexavalent Cr, with an oxidation state of +6 in an alkaline environment, was reduced to hexagonal calcium chromium oxide Ca 5 (CrO4) 3 O 0.5 , determined in the XRD study, with an oxidation state of +5 according to the equation: The other part of Cr (VI) was reduced to the trivalent form of chromium with oxidation state of +3, practically insoluble and chemically inert, rhombohedral Cr 2 O 3 chromium oxide (84-315) according to the equation: XRD studies show that the immobilization of Cr (VI) in SCS was provided by the reaction of a well-soluble salt Na 2 CrO 4 dissolution in water is 84.5 g/100 g at 25 • C) in an alkaline medium with Carbofill E components to form sparingly soluble and chemically inert chromium compounds that are difficult to wash out of soil samples.
The other part of Cr (VI) was reduced to the trivalent form of chromium with oxidation state of +3, practically insoluble and chemically inert, rhombohedral Cr2O3 chromium oxide (84-315) according to the equation: 2CaCrO4 + 4H2O + 6e ̅ → Cr2O3 + CaO + Ca(OH)2 + 6OH − . (3) The other part of Cr (VI) was reduced to the trivalent form of chromium with oxidation state of +3, practically insoluble and chemically inert, rhombohedral Cr2O3 chromium oxide (84-315) according to the equation: (3) XRD studies show that the immobilization of Cr (VI) in SCS was provided b reaction of a well-soluble salt Na2CrO4 dissolution in water is 84.5 g/100 g at 25 °C) alkaline medium with Carbofill E components to form sparingly soluble and chem inert chromium compounds that are difficult to wash out of soil samples.

Conclusions
The self-compacting soils (SCS) were made from sandy and clay soils randoml cavated from a local construction sites using Carbofill E as a binder. The SCS de compressive strength, and water permeability properties produced show that mod soils are a suitable material to achieve the desired properties as designed. When s soil is used, the compressive strength of SCS is higher than that of clay soil, but it is essary to use a higher amount of binder in sandy soil to achieve lower water permeab This study investigated the possibility of immobilizing hexavalent chromium in compacting soils (SCS) using Carbofill E as a binder. Samples of sandy and clay SCS 10, 15, and 20% Carbofill E additives were used in the study; 500 to 100,000 mg of C in the form of Na2CrO4 were added to 1 kg of the SCS sample. Tests showed tha washing of chromium from undisturbed soil samples is more than a hundred times l than that from crushed soil. At the same time, an increase in the amount of Carbo additive in SCS samples reduces the washing out of chromium from them. There when sandy SCS samples with the addition of 10%  15%  20% Carbofill E washed, chromium was washed out of them as follows: 5.87 × 10 −2  0.65 × 10 −2  0 10 −2 mg/kg from uncrushed samples and 18  1.1  0.591 mg/kg. The same chrom washing out relationship was observed from clay SCS samples. According to XRD the crystalline phases of hexagonal calcium chromium oxide Ca5(CrO4)3O0.5 (38-294 rhombohedral chromium oxide Cr2O3 (84-315) were established. Therefore, it is likely most of the chromium in the water-soluble form (Na2CrO4) is converted to practical soluble Ca5(CrO4)3O0.5 and Cr2O3 chromium compounds during the formation of SCS

Conclusions
The self-compacting soils (SCS) were made from sandy and clay soils randomly excavated from a local construction sites using Carbofill E as a binder. The SCS density, compressive strength, and water permeability properties produced show that modified soils are a suitable material to achieve the desired properties as designed. When sandy soil is used, the compressive strength of SCS is higher than that of clay soil, but it is necessary to use a higher amount of binder in sandy soil to achieve lower water permeability.
This study investigated the possibility of immobilizing hexavalent chromium in selfcompacting soils (SCS) using Carbofill E as a binder. Samples of sandy and clay SCS with 10, 15, and 20% Carbofill E additives were used in the study; 500 to 100,000 mg of Cr (VI) in the form of Na 2 CrO 4 were added to 1 kg of the SCS sample. Tests showed that the washing of chromium from undisturbed soil samples is more than a hundred times lower than that from crushed soil. At the same time, an increase in the amount of Carbofill E additive in SCS samples reduces the washing out of chromium from them. Therefore, when sandy SCS samples with the addition of 10% → 15% → 20% Carbofill E were washed, chromium was washed out of them as follows: 5.87 × 10 −2 → 0.65 × 10 −2 → 0.35 × 10 −2 mg/kg from uncrushed samples and 18 → 1.1 → 0.591 mg/kg. The same chromium washing out relationship was observed from clay SCS samples. According to XRD data, the crystalline phases of hexagonal calcium chromium oxide Ca 5 (CrO 4 ) 3 O 0.5  and rhombohedral chromium oxide Cr 2 O 3 (84-315) were established. Therefore, it is likely that most of the chromium in the water-soluble form (Na 2 CrO 4 ) is converted to practically insoluble Ca 5 (CrO 4 ) 3 O 0.5 and Cr 2 O 3 chromium compounds during the formation of SCS samples, which contributes greatly to the efficiency of immobilization. Tests showed that SCSs, regardless of their nature, are suitable for immobilization, since after the samples are washed, more than 99% of the incorporated chromium remains in them. The use of SCS in construction offers the potential to have a significant economic and environmental impact, as well as the potential to immobilize hazardous waste in recycled soil. The effectiveness of the immobilization of individual soils contaminated with hazardous waste (such as petroleum products, hazardous polymeric substances, etc.) should be investigated in future research.

Data Availability Statement:
The data used to support the findings of this study can be made available from the corresponding author upon request.